Arsenic(III) telluride

This This article is full of jargon, which irritates readers who are not experts. Some parts of this article look like a gibberish! may be too technical for most readers to understand. Please help improve it to make it understandable to non-experts, without removing the technical details. (November 2022) (Learn how and when to remove this template message)

|

Arsenic(III) telluride  Identifiers

CAS Number

* 12044-54-1

3D model (JSmol)

* Interactive image

ChemSpider |

* 22797844

EC Number |

* 234-955-1

PubChem CID

* 6336551

InChI

* InChI=1S/2As.3Te

Key: KOOQXSDVIQPGQD-UHFFFAOYSA-N

SMILES

* [As].[As].[Te].[Te].[Te]

Properties

Chemical formula

| As2Te3
Molar mass | 532.64 g·mol−1
Structure[1]

Crystal structure

| Monoclinic

Space group

| C2/m

Lattice constant

a = 14.339 Å, b = 4.006 Å, c = 9.873 Å

α = 90°, β = 95°, γ = 90°

Lattice volume (V)

| 564.96

Formula units (Z)

| 4
Hazards
GHS pictograms |
GHS Signal word | Danger

GHS hazard statements

| H301, H331, H410

GHS precautionary statements

| P261, P264, P270, P271, P273, P301+310, P304+340, P311, P321, P330, P391, P403+233, P405, P501
Related compounds

Other anions

| Arsenic trioxide
Arsenic trisulfide
Arsenic triselenide

Other cations

| Antimony telluride
Bismuth telluride

Except where otherwise noted, data are given for materials in their standard state (at 25 °C [77 °F], 100 kPa).

Infobox references

Arsenic(III) telluride is an inorganic compound with the chemical formula As
2Te
3. It exists in two forms, the monoclinic α phase which transforms under high pressure to a rhombohedral β phase.[2] The compound is a semiconductor, with most current carried by holes.[3] Arsenic telluride has been examined for its use in nonlinear optics.[4]

## Contents

* 1 Molecular and crystal structure
* 2 Applications in nonlinear optics
* 3 Semiconductor
* 4 References

## Molecular and crystal structure

Arsenic(III) telluride is a bulk form[clarification needed] of group 15 sesquichalcogenides[clarification needed] which form chains of As
2Te
3 molecules that are eventually[clarification needed] stacked on top of each other and held together by weak Van der Waals forces.[5] This stacking of long branches of As
2Te
3 molecules gives arsenic(III) telluride an amorphous crystalline[clarification needed] structure that can be found in the ɑ-As
2Te
3 and β-As
2Te
3 configurations at different pressures. At ambient pressure, ɑ-As
2Te
3 yields a monoclinic structure with low thermoelectric properties; however, when placed in high pressure environments, ɑ-As
2Te
3 transforms into the β-As
2Te
3 configuration that has a rhombohedral R3m space group with high thermoelectric properties.[6][clarification needed]

2Te
3 is a semiconductor and has been used to study nonlinear optics due to its ability to conduct electrical current; however, at high temperatures when doped with impurities[which?] causes these conductive abilities to transform irreversibly from its traditional semiconductor ability to metal conduction only.[5][7] This irreversible transformation is most likely caused by the doping materials added to As
2Te
3 forming impurity clusters which causes an increase in paramagnetic tendency of the complex.[5][clarification needed]

## Applications in nonlinear optics

2Te
3 is the least studied amorphous chalcogenide compound, which are a group of semiconductors primarily used in nonlinear optics as glasses or lenses to redistribute light. [8] It has not been studied widely due to the difficulty to synthesize As
2Te
3 into amorphous crystalline solids. In order to avoid crystalizing arsenic telluride, it must be quenched quickly after it comes out of the melt.[8] Arsenic telluride and As
2Te
3 containing materials are starting to increase in popularity in the field of nonlinear optics because the amorphous glasses As
2Te
3 is exceptional at redistributing the electrical charge density of the light source (typically a laser) when it interacts within the medium.[9] The significance of this redistribution is that it allows for the modification of the laser’s nature to perform a specific function. Some examples of this are the use of lasers in sensors, optical communication systems, as well as changing the color of the laser for equipment and other machinery used in materials research.[6][7]

It has also been discovered in recent studies that As
2Te
3 presents mobility edges, which are edges surrounding a conductive gap,[clarification needed] regardless of temperature allowing for the amorphous structure to conduct electricity at greater rates than expected.[8] Due to this, it can be hypothesized that the mobility edges lie between delocalized and localized states as well as having a more energetically efficient transition from dark mobility to photoconductive mobility than other amorphous glasses.[8]

## Semiconductor

Arsenic(III) telluride, in its doped crystalline form, houses electron carriers that are caused by doping impurities that sit close to the edge due to the relatively free electron density around the edges.[10] These relatively free electrons interact with the impurities causing a decrease in electron density around the edge which causes a “tail” to form. These band tails overlap causing a gap or a hole, similar to p-type doping, that can be used for conduction; however, the mobility of the carriers in the lattice decreases significantly near the Fermi level of the two tails.[7][10] This indicates that electronic stimuli, usually phonon related, is needed to induce hopping of electrons into the gap to cause conduction.[5][10] The need of external phonon stimuli to cause electrical conductivity of As
2Te
3 crystals further supports the effectiveness of As
2Te
3 or As
2Te
3 based glasses in the use of nonlinear optics because the light upon entering the lattice causes the electron hopping inducing conduction. Since the electrons are hopping into the conductance gap near the Fermi level, the light is being modified and will exit the lattice in a different form than it entered.[10]

## References

1. ↑ Carron, G. J. (1963-05-01). "The crystal structure and powder data for arsenic telluride". Acta Crystallographica (International Union of Crystallography (IUCr)) 16 (5): 338–343. doi:10.1107/s0365110x63000943. ISSN 0365-110X.
2. ↑ Sharma, Yamini; Srivastava, Pankaj (2011). "First principles investigation of electronic, optical and transport properties of α- and β-phase of arsenic telluride". Optical Materials (Elsevier BV) 33 (6): 899–904. doi:10.1016/j.optmat.2011.01.020. ISSN 0925-3467. Bibcode: 2011OptMa..33..899S.
3. ↑ Moustakas, T. D.; Weiser, K. (1975-09-15). "Transport and recombination properties of amorphous arsenic telluride". Physical Review B (American Physical Society (APS)) 12 (6): 2448–2454. doi:10.1103/physrevb.12.2448. ISSN 0556-2805. Bibcode: 1975PhRvB..12.2448M.
4. ↑ Lee, Jinho; Jhon, Young In; Lee, Kyungtaek; Jhon, Young Min; Lee, Ju Han (2020-09-17). "Nonlinear optical properties of arsenic telluride and its use in ultrafast fiber lasers". Scientific Reports (Springer Science and Business Media LLC) 10 (1): 15305. doi:10.1038/s41598-020-72265-3. ISSN 2045-2322. PMID 32943737. Bibcode: 2020NatSR..1015305L.
5. ↑ 5.0 5.1 5.2 5.3 Biswas, Shipra (2 April 1984). "Anomalous Electrical Resistance in Crystalline As2Te3". Department of Magnetism, Indian Association for the Cultivation of Science.
6. ↑ 6.0 6.1 Lee, Jinho; Jhon, Young In; Lee, Kyungtaek; Jhon, Young Min; Lee, Ju Han (2020-09-17). "Nonlinear optical properties of arsenic telluride and its use in ultrafast fiber lasers" (in en). Scientific Reports 10 (1): 15305. doi:10.1038/s41598-020-72265-3. ISSN 2045-2322. PMID 32943737. Bibcode: 2020NatSR..1015305L.
7. ↑ 7.0 7.1 7.2 Segawa, Hideo (April 1974). "DC and AC Conductivity in Amorphous As2Se3-As2Te3 System". Journal of the Physical Society of Japan 36 (4): 1087–1095. doi:10.1143/jpsj.36.1087. ISSN 0031-9015. Bibcode: 1974JPSJ...36.1087S. http://dx.doi.org/10.1143/jpsj.36.1087.
8. ↑ 8.0 8.1 8.2 8.3 Weiser, K.; Brodsky, M. H. (1970-01-15). "dc Conductivity, Optical Absorption, and Photoconductivity of Amorphous Arsenic Telluride Films". Physical Review B 1 (2): 791–799. doi:10.1103/physrevb.1.791. ISSN 0556-2805. Bibcode: 1970PhRvB...1..791W. http://dx.doi.org/10.1103/physrevb.1.791.
9. ↑ Kityk, I. V.; Kasperczyk, J.; Pluciński, K. (1999-10-01). "Two-photon absorption and photoinduced second-harmonic generation in Sb2Te3–CaCl2–PbCl2 glasses". Journal of the Optical Society of America B 16 (10): 1719. doi:10.1364/josab.16.001719. ISSN 0740-3224. http://dx.doi.org/10.1364/josab.16.001719.
10. ↑ 10.0 10.1 10.2 10.3 Krištofik, J.; Mareš, J. J.; Šmíd, V. (1985-05-16). "The Effect of Pressure on Conductivity and Permittivity of As2Te3-Based Glasses". Physica Status Solidi A 89 (1): 333–345. doi:10.1002/pssa.2210890135. ISSN 0031-8965. Bibcode: 1985PSSAR..89..333K. http://dx.doi.org/10.1002/pssa.2210890135.

* v
* t
* e

Arsenic compounds

* AsBr3
* AsCl3
* AsCl5
* AsF3
* AsF5
* AsH3
* AsHgI4
* AsI3
* As2O3
* As2O5
* As2S3
* As2S5
* As2Se3
* As4S4

0.00

(0 votes)

Original source: https://en.wikipedia.org/wiki/Arsenic(III) telluride. Read more

|

Retrieved from "https://handwiki.org/wiki/index.php?title=Chemistry:Arsenic(III)_telluride&oldid=1077967"
*[CID]: Compound ID
*[H301]: Toxic if swallowed
*[H331]: Toxic if inhaled
*[H410]: Very toxic to aquatic life with long lasting effects
*[P261]: Avoid breathing dust/fume/gas/mist/vapours/spray
*[P264]: Wash … thoroughly after handling
*[P270]: Do not eat, drink or smoke when using this product
*[P271]: Use only outdoors or in a well-ventilated area
*[P273]: Avoid release to the environment
*[P301+310]: IF SWALLOWED: Immediately call a POISON CENTER or doctor/physician
*[P304+340]: IF INHALED: Remove victim to fresh air and keep at rest in a position comfortable for breathing
*[P311]: Call a POISON CENTER or doctor/physician
*[P321]: Specific treatment (see … on this label)
*[P330]: Rinse mouth
*[P391]: Collect spillage
*[P403+233]: Store in a well ventilated place. Keep container tightly closed
*[P405]: Store locked up
*[P501]: Dispose of contents/container to …
*[v]: View this template
*[t]: Discuss this template
*[e]: Edit this template